LMucko/crystallography-open-database huggingface dataset:
Some phases in ternary alloys of Ti, Zr, and Hf, with an Mg As Ag or Al Cu2 Mn type structure
Marazza, R.; Ferro, R.; Rambaldi, G.; Journal of the Less-Common Metals 39 (1975) 341–345; doi:

data_1527754
_publ_section_title
;
 Some phases in ternary alloys of Ti, Zr, and Hf, with an Mg As Ag or Al
 Cu2 Mn type structure
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              341
_journal_page_last               345
_journal_volume                  39
_journal_year                    1975
_chemical_formula_sum            'Hf Pd Sn'
_space_group_IT_number           216
_symmetry_space_group_name_Hall  'F -4 2 3'
_symmetry_space_group_name_H-M   'F -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   6.299
_cell_length_b                   6.299
_cell_length_c                   6.299
_cell_volume                     249.928
_citation_journal_id_ASTM        JCOMAH
_cod_data_source_file            Marazza_JCOMAH_1975_545.cif
_cod_data_source_block           Hf1Pd1Sn1
_cod_original_cell_volume        249.9279
_cod_original_formula_sum        'Hf1 Pd1 Sn1'
_cod_database_code               1527754
Subsolidus equilibria in the ternary aluminium-tin- uranium system
Marazza, R.; Ferro, R.; Mazzone, D.; Rambaldi, G.; Journal of the Less-Common Metals 51 (1977) 51–54; doi:

data_1527755
_publ_section_title
;
 Subsolidus equilibria in the ternary aluminium-tin- uranium system
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              51
_journal_page_last               54
_journal_volume                  51
_journal_year                    1977
_chemical_formula_sum            'Sn3 U'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   4.603
_cell_length_b                   4.603
_cell_length_c                   4.603
_cell_volume                     97.527
_citation_journal_id_ASTM        JCOMAH
_cod_data_source_file            Marazza_JCOMAH_1977_73.cif
_cod_data_source_block           Sn3U1
_cod_original_cell_volume        97.52657
_cod_original_formula_sum        'Sn3 U1'
_cod_database_code               1527755
Ca In2-type and Mg Ag As-type RE Sb Pd compounds (RE= rare earth element)
Marazza, R.; Rossi, D.; Ferro, R.; Journal of the Less-Common Metals 75 (1980) P25–P28; doi:

data_1527756
_publ_section_title
;
 Ca In2-type and Mg Ag As-type RE Sb Pd compounds (RE= rare earth element)
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              P25
_journal_page_last               P28
_journal_volume                  75
_journal_year                    1980
_chemical_formula_sum            'Dy Pd Sb'
_space_group_IT_number           216
_symmetry_space_group_name_Hall  'F -4 2 3'
_symmetry_space_group_name_H-M   'F -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   6.533
_cell_length_b                   6.533
_cell_length_c                   6.533
_cell_volume                     278.829
_citation_journal_id_ASTM        JCOMAH
_cod_data_source_file            Marazza_JCOMAH_1980_434.cif
_cod_data_source_block           Dy1Pd1Sb1
_cod_original_formula_sum        'Dy1 Pd1 Sb1'
_cod_database_code               1527756
Structure cristalline de l'orthostannate de potassium K4 Sn O4
Marchand, R.; Piffard, Y.; Tournoux, M.; Acta Crystallographica B (24,1968-38,1982) 31 (1975) 511–514; doi:

data_2106386
_publ_section_title
;
 Structure cristalline de l'orthostannate de potassium K4 Sn O4
;
_journal_name_full               'Acta Crystallographica B (24,1968-38,1982)'
_journal_page_first              511
_journal_page_last               514
_journal_volume                  31
_journal_year                    1975
_chemical_formula_sum            'K4 O4 Sn'
_chemical_name_systematic        'K4 (Sn O4)'
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                71.82
_cell_angle_beta                 99.89
_cell_angle_gamma                113.13
_cell_formula_units_Z            2
_cell_length_a                   6.48
_cell_length_b                   6.51
_cell_length_c                   9.7
_cell_volume                     356.948
_citation_journal_id_ASTM        ACBCAR
_cod_data_source_file            Marchand_ACBCAR_1975_1667.cif
_cod_data_source_block           K4O4Sn1
_cod_original_cell_volume        356.9483
_cod_original_formula_sum        'K4 O4 Sn1'
_cod_database_code               2106386
Structure cristalline de Eu2(II) Si O4 beta
Marchand, R.; l'Haridon, P.; Laurent, Y.; Journal of Solid State Chemistry 24 (1978) 71–76; doi:

data_1527757
_publ_section_title
;
 Structure cristalline de Eu2(II) Si O4 beta
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              71
_journal_page_last               76
_journal_volume                  24
_journal_year                    1978
_chemical_formula_sum            'Eu2 O4 Si'
_chemical_name_systematic        'Eu2 (Si O4)'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.137
_cell_length_b                   5.665
_cell_length_c                   9.767
_cell_volume                     394.891
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            Marchand_JSSCBI_1978_1242.cif
_cod_data_source_block           Eu2O4Si1
_cod_original_cell_volume        394.8906
_cod_original_formula_sum        'Eu2 O4 Si1'
_cod_database_code               1527757
The V-Sn phase diagram
Marchukova, L.V.; Matveeva, N.M.; Kornilov, I.I.; Izvestiya Akademii Nauk SSSR, Metally 1973 (1973) 157–159; doi:

data_1527758
_publ_section_title
;
 The V-Sn phase diagram
;
_journal_name_full               'Izvestiya Akademii Nauk SSSR, Metally'
_journal_page_first              157
_journal_page_last               159
_journal_volume                  1973
_journal_year                    1973
_chemical_formula_sum            'Sn0.1 V0.9'
_chemical_name_systematic        '(Sn0.1 V0.9)'
_space_group_IT_number           229
_symmetry_space_group_name_Hall  '-I 4 2 3'
_symmetry_space_group_name_H-M   'I m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   3.08
_cell_length_b                   3.08
_cell_length_c                   3.08
_cell_volume                     29.218
_citation_journal_id_ASTM        IZNMAQ
_cod_data_source_file            Marchukova_IZNMAQ_1973_77.cif
_cod_data_source_block           Sn0.1V0.9
_cod_original_cell_volume        29.21811
_cod_database_code               1527758
The Crystal Structure of Ti4 O7, a Member of the Homologous Series Tin O(2n-1)
Marezio, M.; Dernier, P.D.; Journal of Solid State Chemistry 3 (1971) 340–348; doi:

data_1527759
_publ_section_title
;
 The Crystal Structure of Ti4 O7, a Member of the Homologous Series Tin
 O(2n-1)
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              340
_journal_page_last               348
_journal_volume                  3
_journal_year                    1971
_chemical_formula_sum            'O7 Ti4'
_chemical_name_systematic        'Ti4 O7'
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                95.05
_cell_angle_beta                 95.17
_cell_angle_gamma                108.71
_cell_formula_units_Z            4
_cell_length_a                   5.6
_cell_length_b                   7.133
_cell_length_c                   12.466
_cell_volume                     466.096
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            Marezio_JSSCBI_1971_1976.cif
_cod_data_source_block           O7Ti4
_cod_original_cell_volume        466.0957
_cod_database_code               1527759
Superconductivity of ternary sulfides and the structure of Pb Mo6 S8
Marezio, M.; Remeika, J.P.; Dernier, P.D.; Corenzwit, E.; Matthias, B.T.; Materials Research Bulletin 8 (1973) 657–668; doi:

data_1527760
_publ_section_title
;
 Superconductivity of ternary sulfides and the structure of Pb Mo6 S8
;
_journal_name_full               'Materials Research Bulletin'
_journal_page_first              657
_journal_page_last               668
_journal_volume                  8
_journal_year                    1973
_chemical_formula_sum            'Mo6 Pb0.92 S7.5'
_chemical_name_systematic        'Pb0.92 Mo6 S7.5'
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-P 3*'
_symmetry_space_group_name_H-M   'R -3 :R'
_cell_angle_alpha                89.33
_cell_angle_beta                 89.33
_cell_angle_gamma                89.33
_cell_formula_units_Z            1
_cell_length_a                   6.551
_cell_length_b                   6.551
_cell_length_c                   6.551
_cell_volume                     281.083
_citation_journal_id_ASTM        MRBUAC
_cod_data_source_file            Marezio_MRBUAC_1973_1273.cif
_cod_data_source_block           Mo6Pb0.92S7.5
_cod_original_cell_volume        281.0829
_cod_original_sg_symbol_Hall     '-R 3 (-y+z,x+z,-x+y+z)'
_cod_database_code               1527760
Low-temperature X-ray diffraction studies of near-equiatomic V Ru alloys
Marezio, M.; Dernier, P.D.; Chu, C.W.; Physical Review, Serie 3. B - Condensed Matter (18,1978-) 4 (1971) 2825–2826; doi:

data_1527761
_publ_section_title
;
 Low-temperature X-ray diffraction studies of near-equiatomic V Ru alloys
;
_journal_name_full
'Physical Review, Serie 3. B - Condensed Matter (18,1978-)'
_journal_page_first              2825
_journal_page_last               2826
_journal_volume                  4
_journal_year                    1971
_chemical_formula_sum            'Ru V'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   2.99
_cell_length_b                   2.99
_cell_length_c                   2.99
_cell_volume                     26.731
_citation_journal_id_ASTM        PRBMDO
_cod_data_source_file            Marezio_PRBMDO_1971_9.cif
_cod_data_source_block           Ru1V1
_cod_original_cell_volume        26.7309
_cod_original_formula_sum        'Ru1 V1'
_cod_database_code               1527761
Investigations on a New Copper Niobium Oxide of Li Nb3 O8 Type Using Chemical Analysis and X-Ray Powder Diffraction Profile Analysis
Marinder, B.O.; Werner, P.E.; Wahlstroem, E.; Malmros, G.; Acta Chemica Scandinavica, Series A: (28,1974-) 34 (1980) 51–56; doi:

data_1527762
_publ_section_title
;
 Investigations on a New Copper Niobium Oxide of Li Nb3 O8 Type Using
 Chemical Analysis and X-Ray Powder Diffraction Profile Analysis
;
_journal_name_full
'Acta Chemica Scandinavica, Series A: (28,1974-)'
_journal_page_first              51
_journal_page_last               56
_journal_volume                  34
_journal_year                    1980
_chemical_formula_sum            'Cu Nb3 O8'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2yab'
_symmetry_space_group_name_H-M   'P 1 21/a 1'
_cell_angle_alpha                90
_cell_angle_beta                 107.18
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   15.365
_cell_length_b                   5.0717
_cell_length_c                   7.5266
_cell_volume                     560.353
_citation_journal_id_ASTM        ACAPCT
_cod_data_source_file            Marinder_ACAPCT_1980_909.cif
_cod_data_source_block           Cu1Nb3O8
_cod_original_cell_volume        560.3531
_cod_original_sg_symbol_Hall     '-P 2ybc (z,y,-x)'
_cod_original_formula_sum        'Cu1 Nb3 O8'
_cod_database_code               1527762
Erstmalige Fixierung des instabilen Schwefelmonoxids in einem Cluster: Synthese und Struktur von Fe3 (C O)9 (S) S O
Marko, L.; Marko-Monostory, B.; Madach, T.; Vahrenkamp, H.; Angewandte Chemie (German Edition) 92 (1980) 225–226; doi:

data_1527763
_publ_section_title
;
 Erstmalige Fixierung des instabilen Schwefelmonoxids in einem Cluster:
 Synthese und Struktur von Fe3 (C O)9 (S) S O
;
_journal_name_full               'Angewandte Chemie (German Edition)'
_journal_page_first              225
_journal_page_last               226
_journal_volume                  92
_journal_year                    1980
_chemical_formula_sum            'C9 Fe3 O10 S2'
_chemical_name_systematic        'Fe3 (C O)9 (S) S O'
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                91.38
_cell_angle_beta                 116.97
_cell_angle_gamma                97.06
_cell_formula_units_Z            2
_cell_length_a                   9.514
_cell_length_b                   10.32
_cell_length_c                   9.065
_cell_volume                     784.018
_citation_journal_id_ASTM        ANCEAD
_cod_data_source_file            Marko_ANCEAD_1980_896.cif
_cod_data_source_block           C9Fe3O10S2
_cod_original_cell_volume        784.0179
_cod_database_code               1527763
The crystal structure of potassium pentathionate hemitrihydrate
Maroy, K.; Acta Chemica Scandinavica (1-27,1973-42,1988) 25 (1971) 2580–2590; doi:

data_1527764
_publ_section_title
;
 The crystal structure of potassium pentathionate hemitrihydrate
;
_journal_name_full               'Acta Chemica Scandinavica (1-27,1973-42,1988)'
_journal_page_first              2580
_journal_page_last               2590
_journal_volume                  25
_journal_year                    1971
_chemical_formula_sum            'H3 K2 O7.5 S5'
_chemical_name_systematic        'K2 (S3 (S O3)2) (H2 O)1.5'
_space_group_IT_number           60
_symmetry_space_group_name_Hall  '-P 2n 2ab'
_symmetry_space_group_name_H-M   'P b c n'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   20.316
_cell_length_b                   9.229
_cell_length_c                   12.248
_cell_volume                     2296.455
_citation_journal_id_ASTM        ACSAA4
_cod_data_source_file            Maroy_ACSAA4_1971_1191.cif
_cod_data_source_block           H3K2O7.5S5
_cod_original_cell_volume        2296.456
_cod_database_code               1527764
The crystal structure of rubidium telluropentathionate hemitrihydrate
Maroy, K.; Acta Chemica Scandinavica (1-27,1973-42,1988) 25 (1971) 2557–2568; doi:

data_1527765
_publ_section_title
;
 The crystal structure of rubidium telluropentathionate hemitrihydrate
;
_journal_name_full
'Acta Chemica Scandinavica (1-27,1973-42,1988)'
_journal_page_first              2557
_journal_page_last               2568
_journal_volume                  25
_journal_year                    1971
_chemical_formula_sum            'H3 O7.5 Rb2 S4 Te'
_chemical_name_systematic        'Rb2 (Te (S2 O3)2) (H2 O)1.5'
_space_group_IT_number           60
_symmetry_space_group_name_Hall  '-P 2n 2ab'
_symmetry_space_group_name_H-M   'P b c n'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   21.32
_cell_length_b                   9.446
_cell_length_c                   12.437
_cell_volume                     2504.672
_citation_journal_id_ASTM        ACSAA4
_cod_data_source_file            Maroy_ACSAA4_1971_1193.cif
_cod_data_source_block           H3O7.5Rb2S4Te1
_cod_original_formula_sum        'H3 O7.5 Rb2 S4 Te1'
_cod_database_code               1527765
The Crystal Structure of Barium Selenopentationate Trihydrate
Maroy, K.; Acta Chemica Scandinavica (1-27,1973-42,1988) 26 (1972) 45–58; doi:

data_1527766
_publ_section_title
;
 The Crystal Structure of Barium Selenopentationate Trihydrate
;
_journal_name_full               'Acta Chemica Scandinavica (1-27,1973-42,1988)'
_journal_page_first              45
_journal_page_last               58
_journal_volume                  26
_journal_year                    1972
_chemical_formula_sum            'Ba H5.08 O8.54 S4 Se'
_chemical_name_systematic        'Ba Se (S2 O3)2 (H2 O)2.54'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 110.85
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   10.502
_cell_length_b                   4.992
_cell_length_c                   23.987
_cell_volume                     1175.192
_citation_journal_id_ASTM        ACSAA4
_cod_data_source_file            Maroy_ACSAA4_1972_963.cif
_cod_data_source_block           H5.08Ba1O8.54S4Se1
_cod_original_cell_volume        1175.193
_cod_original_formula_sum        'H5.08 Ba1 O8.54 S4 Se1'
_cod_database_code               1527766
Refinement of the Crystal Structure of Barium Selenopentathionate Dihydrate
Maroy, K.; Acta Chemica Scandinavica (1-27,1973-42,1988) 26 (1972) 36–44; doi:

data_1527767
_publ_section_title
;
 Refinement of the Crystal Structure of Barium Selenopentathionate
 Dihydrate
;
_journal_name_full               'Acta Chemica Scandinavica (1-27,1973-42,1988)'
_journal_page_first              36
_journal_page_last               44
_journal_volume                  26
_journal_year                    1972
_chemical_formula_sum            'Ba H3.5 O7.75 S4 Se'
_chemical_name_systematic        'Ba Se (S2 O3)2 (H2 O)1.75'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.043
_cell_length_b                   10.434
_cell_length_c                   22.372
_cell_volume                     1177.185
_citation_journal_id_ASTM        ACSAA4
_cod_data_source_file            Maroy_ACSAA4_1972_964.cif
_cod_data_source_block           H3.5Ba1O7.75S4Se1
_cod_original_formula_sum        'H3.5 Ba1 O7.75 S4 Se1'
_cod_database_code               1527767
Refinement of the Crystal Structure of Monoclinic Barium Telluropentathionate Dihydrate
Maroy, K.; Acta Chemica Scandinavica (1-27,1973-42,1988) 27 (1973) 1695–1704; doi:

data_1527768
_publ_section_title
;
 Refinement of the Crystal Structure of Monoclinic Barium
 Telluropentathionate Dihydrate
;
_journal_name_full
'Acta Chemica Scandinavica (1-27,1973-42,1988)'
_journal_page_first              1695
_journal_page_last               1704
_journal_volume                  27
_journal_year                    1973
_chemical_formula_sum            'Ba H2.52 O7.26 S4 Te'
_chemical_name_systematic        'Ba Te (S2 O3)2 (H2 O)1.26'
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-A 2y'
_symmetry_space_group_name_H-M   'A 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 98.61
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.003
_cell_length_b                   10.588
_cell_length_c                   23.635
_cell_volume                     1237.878
_citation_journal_id_ASTM        ACSAA4
_cod_data_source_file            Maroy_ACSAA4_1973_845.cif
_cod_data_source_block           H2.52Ba1O7.26S4Te1
_cod_original_sg_symbol_Hall     '-C 2y (z,y,-x)'
_cod_original_formula_sum        'H2.52 Ba1 O7.26 S4 Te1'
_cod_database_code               1527768
Zur Kenntnis von K2 Pb2 O3
Martens, K.P.; Hoppe, R.; Zeitschrift fuer Anorganische und Allgemeine Chemie 437 (1977) 116–122; doi:

data_1527769
_publ_section_title
;
 Zur Kenntnis von K2 Pb2 O3
;
_journal_name_full
'Zeitschrift fuer Anorganische und Allgemeine Chemie'
_journal_page_first              116
_journal_page_last               122
_journal_volume                  437
_journal_year                    1977
_chemical_formula_sum            'K2 O3 Pb2'
_chemical_name_systematic        'K2 Pb2 O3'
_space_group_IT_number           199
_symmetry_space_group_name_Hall  'I 2b 2c 3'
_symmetry_space_group_name_H-M   'I 21 3'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   8.419
_cell_length_b                   8.419
_cell_length_c                   8.419
_cell_volume                     596.735
_citation_journal_id_ASTM        ZAACAB
_cod_data_source_file            Martens_ZAACAB_1977_926.cif
_cod_data_source_block           K2O3Pb2
_cod_original_cell_volume        596.7349
_cod_database_code               1527769
Das erste Oxoplumbat(II) mit Inselstruktur: K4 Pb O3
Martens, K.P.; Hoppe, R.; Zeitschrift fuer Anorganische und Allgemeine Chemie 438 (1978) 105–114; doi:

data_1527770
_publ_section_title
;
 Das erste Oxoplumbat(II) mit Inselstruktur: K4 Pb O3
;
_journal_name_full
'Zeitschrift fuer Anorganische und Allgemeine Chemie'
_journal_page_first              105
_journal_page_last               114
_journal_volume                  438
_journal_year                    1978
_chemical_formula_sum            'K4 O3 Pb'
_chemical_name_systematic        'K4 Pb O3'
_space_group_IT_number           61
_symmetry_space_group_name_Hall  '-P 2ac 2ab'
_symmetry_space_group_name_H-M   'P b c a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   6.543
_cell_length_b                   11.405
_cell_length_c                   18.709
_cell_volume                     1396.120
_citation_journal_id_ASTM        ZAACAB
_cod_data_source_file            Martens_ZAACAB_1978_1591.cif
_cod_data_source_block           K4O3Pb1
_cod_original_cell_volume        1396.12
_cod_original_formula_sum        'K4 O3 Pb1'
_cod_database_code               1527770
Synthesis and X-Ray Crystal Structure of the (Rh5 (C O)8 (Mue-C O)6 I)(2-) Anion Containing A Trigonal Bipyramidal Rhodium Cluster
Martinengo, S.; Ciani, G.; Sironi, A.; Journal of the Chemical Society. Chemical Communications (1972-) 1979 (1979) 1059–1061; doi:

data_7117492
_publ_section_title
;
 Synthesis and X-Ray Crystal Structure of the (Rh5 (C O)8 (Mue-C O)6
 I)(2-) Anion Containing A Trigonal Bipyramidal Rhodium Cluster
;
_journal_name_full
;
Journal of the Chemical Society. Chemical Communications (1972-)
;
_journal_page_first              1059
_journal_page_last               1061
_journal_volume                  1979
_journal_year                    1979
_chemical_formula_sum            'C44 I N2 O14 Rh5'
_chemical_name_systematic        '((C4 H9)4 N)2 (Rh5 (C O)14 I)'
_space_group_IT_number           33
_symmetry_space_group_name_Hall  'P -2ac -2n'
_symmetry_space_group_name_H-M   'P n 21 a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   27.767
_cell_length_b                   18.652
_cell_length_c                   11.678
_cell_volume                     6048.154
_citation_journal_id_ASTM        JCCCAT
_cod_data_source_file            Martinengo_JCCCAT_1979_868.cif
_cod_data_source_block           C44I1N2O14Rh5
_cod_original_sg_symbol_Hall     'P 2c -2n (-x,z,y)'
_cod_original_formula_sum        'C44 I1 N2 O14 Rh5'
_cod_database_code               7117492